Chapter 5 Microcontact printing methods for molecular ... Microcontact printing methods for...
Embed Size (px)
Transcript of Chapter 5 Microcontact printing methods for molecular ... Microcontact printing methods for...
Microcontact printing methods for molecular
Microcontact printing (μCP) is a highly
versatile technique for patterning surfaces
using monolayers with submicron resolution.1
Like other soft lithography techniques, μCP is
based on replicating a pattern from a flexible,
elastomeric stamp to a surface. In this method,
the pattern is transferred by coating the stamp
with a molecule capable of forming a covalent
bond with the surface and forming an intimate
contact between the two materials (Figure
Figure 5.1. Schematic of microcontact printing. A. A PDMS stamp coated with an ink solution is brought into contact with a substrate. B. The ink covalently attaches to the substrate and the stamp is removed.
117 5.1A). Due to high local concentration of the molecules, a monolayer rapidly forms on
the surface, replicating the pattern on the stamp (Figure 5.1B).
There are several applications for μCP. As an alternative to conventional
lithography, μCP has been used to pattern self-assembled monolayers (SAMs) as
ultrathin wet etch resists2, 3 and as templates for the growth or deposition of materials4.
The flexible nature of the elastomeric stamp also facilitates the patterning on non-planar
surfaces, leading to applications in a variety of fields including optics and MEMS.1
The key to μCP’s success is in its highly simple, high throughput and inexpensive
nature. μCP is a bottom-up fabrication technique. Since surface structures are added, not
removed, very little waste is generated. Conventional lithography, in contrast, consists of
applying a resist and then removing patterns from it. Both the resist and the resist
developer are toxic chemicals and generate hazardous waste. Another benefit to μCP is
that very large areas can be patterned easily by using a large planar stamp or a rolling
stamp (analogous to a paint roller).1 Standard lithography techniques become
progressively more expensive as the exposure area increases. Lastly, the materials
involved with μCP: the elastomer stamp (typically polydimethylsiloxane), the ink
molecule, and the ink solvent (usually a standard solvent in organic synthesis like
acetonitrile) are all inexpensive and quick to assemble. In contrast, the instruments,
facilities, and masks used in conventional lithography are very expensive and require
specialized training. Thus, μCP is a promising technique for micro- and nanofabrication.
Recently, μCP has been used to facilitate covalent attachments of new molecules
to existing SAMs using chemistries such as Cu-catalyzed azide-alkyne cycloaddition, 5, 6
imine bond formation,7–9 and amide bond formation.10–12 In this technique, molecules are
118 stamped on an existing monolayer. The highly confined interface between the stamp and
the substrate promotes a reaction between the ink and monolayer, often times with
reaction rates much faster than the analogous solution-based reaction and without an
added catalyst.11 This methdology has been used to pattern oligonucleotides for
microassays and biosensors,6, 9 immobilize cells to study cell-cell and cell-surface
interactions,8 generate peptide arrays for proteins studies,11 and biological ligands for
immunoassays and biosensors.12
5.1.1 Application for high-density molecular circuits
Covalent surface attachment using μCP has
great potential for applications outside of biology
as well. In particular, it may be a useful tool in the
fabrication of high-density molecular circuits. In
2007, Green et al. described a molecular electronic
circuit using a silicon nanowire (Si NW) crossbar
array and a monolayer of amphiphilic, bistable
rotaxanes as the active memory element.13 The
development of Si NW devices14 and circuits15 was
described in Chapters 2–4.
The rotaxanes, assembled in molecular
switch tunnel junctions (MSTJs), have been shown
to switch between a low conductance state and a
high conductance state by the mechanical shuttle of
Figure 5.2. Molecular structure of a amphiphilic, bistable rotaxane
119 the tetracationic cyclophane ring (shown in blue in Figure 5.2) from the tetrathiafulvalene
site (shown in green) to the dioxynapthalene site (shown in red).16, 17 This mechanical
shuttle occurs when the tetrathiafulvalene (TTF) group is oxidized by applying a large
bias across the solid-state device electrodes. The current levels are then “read” by
applying a small, non-perturbing bias.
Although the rotaxane memory devices have been successfully demonstrated,
the integration of the monolayer into the device has to be done carefully.18 The
rotaxanes are compressed and aligned via the Langmuir-Blodgett technique and
transferred to the bottom electrodes of the memory circuit. The top electrodes are then
carefully deposited on top of the monolayer. If the monolayer is compressed at the
wrong pressure, the MSTJ fails. Also, the use of the Langmuir-Blodgett technique places
design constraints on the molecule and the substrate and the molecules are not covalently
attached to the electrodes.
μCP would be a convenient alternative to the Langmuir-Blodgett method for
patterning molecular electronic devices directly onto electrode surfaces. This technique
has the benefit that the attachment would be covalent, which may lead to better device
performance and longer performance times. For instance, this technique may allow the
sequential, solvent-free synthesis of rotaxanes directly on devices. Figure 5.3 shows a
proposed synthetic sequence. The rotaxane backbone containing the TTF and
dioxynapthalene (DNP) sites would be covalently attached to the surface using μCP. The
tetracationic cyclophane ring (CBPQT4+) would be stamped next, and the electrostatic
interactions between the ring and the rotaxane backbone would promote a threading
120 process. The stopper (which prevents the ring from slipping off the backbone) would
then be stamped and covalently attached.
This proposed synthesis would allow for the rapid fabrication of both the
molecule and device simultaneously. This process would be extremely fast, be high
yielding, and generate little waste. Unlike the Langmuir-Blodgett technique, the
monolayer would be covalently attached to the surface and also could be patterned into
the desired device geometry. Advances in the nanoimprint lithography of nanowires19
would provide a complement to this technology and be an attractive method for the high-
throughput generation of novel nanoscale and molecule-based electronic circuits.
Figure 5.3. Schematic of proposed rotaxane synthesis. The rotaxane backbone would first be covalently attached by μCP. The tetracationic cyclophane ring (CBPQT4+) and the stopper would be also sequentially stamped, forming the complete rotaxane on the electrode surface.
121 5.1.2 Organization of the chapter
This chapter describes the work done on developing μCP methods for the CuI-
catalyzed azide-alkyne cycloaddition (CuAAC) reaction on Au and Si substrates.
Because alkanethiol monolayers on Au are the best characterized SAM system,20 the
majority of the results were obtained using these substrates. μCP was shown to work
using both homogeneous and heterogeneous Cu catalysts. The use of the heterogeneous
catalyst for μCP was a novel result and its kinetics and mechanism were explored in
In the next two sections, the stamping process and the surface characterization
experimental methods are described. Then, the results of the surface characterization are
discussed, followed by discussions of the kinetics of the stamping process using the
homogeneous and heterogeneous stamps and the mechanism for μCP using the
heterogeneous catalyst. Lastly, the generation of azide-terminated silicon surfaces is
described, along with preliminary stamping results.
122 5.2 Generation of azide-terminated monolayers on Au
Mixed monolayers consisting of 50% azide termination and 50% methyl
termination were prepared by immersing Au substrates into a 1 mM solution of 50%
octanethiol and 50% 1-azido-11-undecanethiol in ethanol. Au surfaces were prepared by
depositing 15/150 nm Ti/Au on clean, 4-inch Si(100) wafers. The wafers were cleaved
into 1.5 × 1.5 cm2 pieces and cleaned via a one minute soak in hot acid piranha (3:1
H2SO4: 30% H2O2), followed by a 15 second immersion in H2O and a 15 second
immersion in concentrated HCl at room temperature. The pieces were then rinsed with
DI H2O and EtOH, and were immediately placed in the thiol solution for 16–36 hours.
The reaction was protected from light to prevent photo-oxidation of the thi